#------------------------------------------------------------------------------
#$Date: 2021-04-09 10:52:39 +0300 (Fri, 09 Apr 2021) $
#$Revision: 264004 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/15/1561594.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561594
loop_
_publ_author_name
'Latshaw, Allison M.'
'Yeon, Jeongho'
'Smith, Mark D.'
'zur Loye, Hans-Conrad'
_publ_section_title
;
 Synthesis, structure, and polymorphism of A3LnSi2O7 (A=Na, K; Ln=Sm, Ho,
 Yb)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              100
_journal_page_last               106
_journal_paper_doi               10.1016/j.jssc.2015.12.013
_journal_volume                  235
_journal_year                    2016
_chemical_formula_moiety         'K3 O7 Si2 Sm'
_chemical_formula_sum            'K3 O7 Si2 Sm'
_chemical_formula_weight         435.83
_space_group_crystal_system      hexagonal
_space_group_IT_number           193
_space_group_name_Hall           '-P 6c 2'
_space_group_name_H-M_alt        'P 63/m c m'
_atom_sites_solution_hydrogens   .
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.97640(10)
_cell_length_b                   9.97640(10)
_cell_length_c                   14.4844(3)
_cell_measurement_reflns_used    7870
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      35.080
_cell_measurement_theta_min      2.812
_cell_volume                     1248.47(3)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.631 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0363
_diffrn_reflns_av_unetI/netI     0.0125
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            28791
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         35.267
_diffrn_reflns_theta_min         2.357
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    8.842
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6204
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.478
_exptl_crystal_description       prism
_exptl_crystal_F_000             1218
_exptl_crystal_size_max          0.140
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_refine_diff_density_max         1.035
_refine_diff_density_min         -0.784
_refine_diff_density_rms         0.166
_refine_ls_extinction_coef       0.00074(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.184
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     41
_refine_ls_number_reflns         1047
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.184
_refine_ls_R_factor_all          0.0354
_refine_ls_R_factor_gt           0.0279
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0354P)²+2.4953P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0733
_refine_ls_wR_factor_ref         0.0766
_reflns_number_gt                881
_reflns_number_total             1047
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            mmc1.cif
_cod_data_source_block           K3SmSi2O7
_cod_original_cell_volume        1248.47(4)
_cod_database_code               1561594
_shelx_space_group_comment
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;
_shelx_estimated_absorpt_t_min   0.371
_shelx_estimated_absorpt_t_max   0.538
_shelxl_version_number           2013-4
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.0000 0.0000 0.2500 0.00712(11) Uani 1 12 d S T P . .
Sm2 Sm 0.3333 0.6667 0.0000 0.00729(10) Uani 1 6 d S T P . .
K1 K 0.33091(8) 0.0000 0.09067(6) 0.02001(18) Uani 1 2 d S T P . .
K2 K 0.3333 0.6667 0.2500 0.0189(3) Uani 1 6 d S T P . .
K3 K 0.0000 0.0000 0.0000 0.0174(4) Uani 1 12 d S T P . .
Si1 Si 0.65878(8) 0.0000 0.14352(6) 0.00733(17) Uani 1 2 d S T P . .
O1 O 0.6782(2) 0.5249(2) 0.90624(13) 0.0165(4) Uani 1 1 d . . . . .
O2 O 0.8216(2) 0.0000 0.14536(16) 0.0134(4) Uani 1 2 d S T P . .
O3 O 0.5975(4) 0.0000 0.2500 0.0151(7) Uani 1 4 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sm Sm -0.1638 3.4418 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Sm1 O2 135.24(4) 18_666 2_545
O2 Sm1 O2 135.24(4) 18_666 1_455
O2 Sm1 O2 82.51(9) 2_545 1_455
O2 Sm1 O2 80.82(12) 18_666 3_665
O2 Sm1 O2 82.51(9) 2_545 3_665
O2 Sm1 O2 82.51(9) 1_455 3_665
O2 Sm1 O2 82.51(9) 18_666 17_546
O2 Sm1 O2 80.82(12) 2_545 17_546
O2 Sm1 O2 135.24(4) 1_455 17_546
O2 Sm1 O2 135.24(4) 3_665 17_546
O2 Sm1 O2 82.51(9) 18_666 16_456
O2 Sm1 O2 135.24(4) 2_545 16_456
O2 Sm1 O2 80.82(12) 1_455 16_456
O2 Sm1 O2 135.24(4) 3_665 16_456
O2 Sm1 O2 82.51(9) 17_546 16_456
O2 Sm1 K3 130.41(6) 18_666 .
O2 Sm1 K3 49.59(6) 2_545 .
O2 Sm1 K3 49.59(6) 1_455 .
O2 Sm1 K3 49.59(6) 3_665 .
O2 Sm1 K3 130.41(6) 17_546 .
O2 Sm1 K3 130.41(6) 16_456 .
O2 Sm1 K3 49.59(6) 18_666 4
O2 Sm1 K3 130.41(6) 2_545 4
O2 Sm1 K3 130.41(6) 1_455 4
O2 Sm1 K3 130.41(6) 3_665 4
O2 Sm1 K3 49.59(6) 17_546 4
O2 Sm1 K3 49.59(6) 16_456 4
K3 Sm1 K3 180.0 . 4
O2 Sm1 K1 174.55(6) 18_666 3
O2 Sm1 K1 46.887(15) 2_545 3
O2 Sm1 K1 46.887(15) 1_455 3
O2 Sm1 K1 104.64(6) 3_665 3
O2 Sm1 K1 93.40(4) 17_546 3
O2 Sm1 K1 93.40(4) 16_456 3
K3 Sm1 K1 55.045(13) . 3
K3 Sm1 K1 124.955(13) 4 3
O2 Sm1 K1 46.887(15) 18_666 16_556
O2 Sm1 K1 93.40(4) 2_545 16_556
O2 Sm1 K1 174.55(6) 1_455 16_556
O2 Sm1 K1 93.40(4) 3_665 16_556
O2 Sm1 K1 46.888(15) 17_546 16_556
O2 Sm1 K1 104.64(6) 16_456 16_556
K3 Sm1 K1 124.955(13) . 16_556
K3 Sm1 K1 55.045(13) 4 16_556
K1 Sm1 K1 131.615(8) 3 16_556
O2 Sm1 K1 46.887(15) 18_666 17_556
O2 Sm1 K1 174.55(6) 2_545 17_556
O2 Sm1 K1 93.40(4) 1_455 17_556
O2 Sm1 K1 93.40(4) 3_665 17_556
O2 Sm1 K1 104.64(6) 17_546 17_556
O2 Sm1 K1 46.888(15) 16_456 17_556
K3 Sm1 K1 124.955(13) . 17_556
K3 Sm1 K1 55.045(13) 4 17_556
K1 Sm1 K1 131.615(8) 3 17_556
K1 Sm1 K1 90.437(18) 16_556 17_556
O2 Sm1 K1 104.64(6) 18_666 18_556
O2 Sm1 K1 93.40(4) 2_545 18_556
O2 Sm1 K1 93.40(4) 1_455 18_556
O2 Sm1 K1 174.55(6) 3_665 18_556
O2 Sm1 K1 46.888(15) 17_546 18_556
O2 Sm1 K1 46.888(15) 16_456 18_556
K3 Sm1 K1 124.955(13) . 18_556
K3 Sm1 K1 55.045(13) 4 18_556
K1 Sm1 K1 69.91(3) 3 18_556
K1 Sm1 K1 90.437(18) 16_556 18_556
K1 Sm1 K1 90.437(18) 17_556 18_556
O1 Sm2 O1 87.94(9) 24_664 15_556
O1 Sm2 O1 88.69(7) 24_664 23_564
O1 Sm2 O1 94.90(9) 15_556 23_564
O1 Sm2 O1 94.90(9) 24_664 14_566
O1 Sm2 O1 88.69(7) 15_556 14_566
O1 Sm2 O1 175.02(9) 23_564 14_566
O1 Sm2 O1 88.69(7) 24_664 22_554
O1 Sm2 O1 175.02(9) 15_556 22_554
O1 Sm2 O1 88.69(7) 23_564 22_554
O1 Sm2 O1 87.94(9) 14_566 22_554
O1 Sm2 O1 175.02(9) 24_664 13_666
O1 Sm2 O1 88.69(7) 15_556 13_666
O1 Sm2 O1 87.94(9) 23_564 13_666
O1 Sm2 O1 88.69(7) 14_566 13_666
O1 Sm2 O1 94.90(9) 22_554 13_666
O1 Sm2 K1 50.94(5) 24_664 14_565
O1 Sm2 K1 57.72(5) 15_556 14_565
O1 Sm2 K1 56.50(5) 23_564 14_565
O1 Sm2 K1 128.48(5) 14_566 14_565
O1 Sm2 K1 122.24(5) 22_554 14_565
O1 Sm2 K1 124.08(5) 13_666 14_565
O1 Sm2 K1 57.72(5) 24_664 1_565
O1 Sm2 K1 50.94(5) 15_556 1_565
O1 Sm2 K1 128.48(5) 23_564 1_565
O1 Sm2 K1 56.50(5) 14_566 1_565
O1 Sm2 K1 124.08(5) 22_554 1_565
O1 Sm2 K1 122.24(5) 13_666 1_565
K1 Sm2 K1 72.05(3) 14_565 1_565
O1 Sm2 K1 56.50(5) 24_664 13_665
O1 Sm2 K1 124.08(5) 15_556 13_665
O1 Sm2 K1 122.24(5) 23_564 13_665
O1 Sm2 K1 57.72(5) 14_566 13_665
O1 Sm2 K1 50.94(5) 22_554 13_665
O1 Sm2 K1 128.48(5) 13_666 13_665
K1 Sm2 K1 107.390(15) 14_565 13_665
K1 Sm2 K1 73.18(2) 1_565 13_665
O1 Sm2 K1 124.08(5) 24_664 2
O1 Sm2 K1 56.50(5) 15_556 2
O1 Sm2 K1 57.72(5) 23_564 2
O1 Sm2 K1 122.24(5) 14_566 2
O1 Sm2 K1 128.48(5) 22_554 2
O1 Sm2 K1 50.94(5) 13_666 2
K1 Sm2 K1 73.18(2) 14_565 2
K1 Sm2 K1 107.390(15) 1_565 2
K1 Sm2 K1 179.33(2) 13_665 2
O1 Sm2 K1 128.48(5) 24_664 3_665
O1 Sm2 K1 122.24(5) 15_556 3_665
O1 Sm2 K1 124.08(5) 23_564 3_665
O1 Sm2 K1 50.94(5) 14_566 3_665
O1 Sm2 K1 57.72(5) 22_554 3_665
O1 Sm2 K1 56.50(5) 13_666 3_665
K1 Sm2 K1 179.33(2) 14_565 3_665
K1 Sm2 K1 107.390(15) 1_565 3_665
K1 Sm2 K1 72.05(3) 13_665 3_665
K1 Sm2 K1 107.390(15) 2 3_665
O1 Sm2 K1 122.24(5) 24_664 15
O1 Sm2 K1 128.48(5) 15_556 15
O1 Sm2 K1 50.94(5) 23_564 15
O1 Sm2 K1 124.08(5) 14_566 15
O1 Sm2 K1 56.50(5) 22_554 15
O1 Sm2 K1 57.72(5) 13_666 15
K1 Sm2 K1 107.390(15) 14_565 15
K1 Sm2 K1 179.33(2) 1_565 15
K1 Sm2 K1 107.390(15) 13_665 15
K1 Sm2 K1 72.05(3) 2 15
K1 Sm2 K1 73.18(2) 3_665 15
O1 K1 O1 172.88(8) 15_546 10_666
O1 K1 O2 55.17(6) 15_546 2_545
O1 K1 O2 117.73(6) 10_666 2_545
O1 K1 O2 117.73(6) 15_546 3_665
O1 K1 O2 55.17(6) 10_666 3_665
O2 K1 O2 62.56(9) 2_545 3_665
O1 K1 O1 119.54(2) 15_546 12_556
O1 K1 O1 67.30(7) 10_666 12_556
O2 K1 O1 162.47(6) 2_545 12_556
O2 K1 O1 119.76(5) 3_665 12_556
O1 K1 O1 67.30(7) 15_546 14_556
O1 K1 O1 119.54(2) 10_666 14_556
O2 K1 O1 119.76(5) 2_545 14_556
O2 K1 O1 162.47(6) 3_665 14_556
O1 K1 O1 52.25(7) 12_556 14_556
O1 K1 O1 66.10(6) 15_546 24_654
O1 K1 O1 117.37(4) 10_666 24_654
O2 K1 O1 100.78(6) 2_545 24_654
O2 K1 O1 129.56(6) 3_665 24_654
O1 K1 O1 90.35(6) 12_556 24_654
O1 K1 O1 67.94(6) 14_556 24_654
O1 K1 O1 117.37(4) 15_546 2_654
O1 K1 O1 66.10(6) 10_666 2_654
O2 K1 O1 129.56(6) 2_545 2_654
O2 K1 O1 100.78(6) 3_665 2_654
O1 K1 O1 67.94(6) 12_556 2_654
O1 K1 O1 90.35(6) 14_556 2_654
O1 K1 O1 51.35(7) 24_654 2_654
O1 K1 Si1 93.14(4) 15_546 .
O1 K1 Si1 93.14(4) 10_666 .
O2 K1 Si1 136.87(5) 2_545 .
O2 K1 Si1 136.87(5) 3_665 .
O1 K1 Si1 28.66(3) 12_556 .
O1 K1 Si1 28.66(3) 14_556 .
O1 K1 Si1 89.12(4) 24_654 .
O1 K1 Si1 89.12(4) 2_654 .
O1 K1 Si1 91.03(4) 15_546 13_655
O1 K1 Si1 91.03(4) 10_666 13_655
O2 K1 Si1 106.93(5) 2_545 13_655
O2 K1 Si1 106.93(5) 3_665 13_655
O1 K1 Si1 89.29(4) 12_556 13_655
O1 K1 Si1 89.29(4) 14_556 13_655
O1 K1 Si1 28.33(3) 24_654 13_655
O1 K1 Si1 28.33(3) 2_654 13_655
Si1 K1 Si1 101.43(3) . 13_655
O1 K1 Si1 27.53(4) 15_546 2_545
O1 K1 Si1 145.47(5) 10_666 2_545
O2 K1 Si1 28.15(5) 2_545 2_545
O2 K1 Si1 90.47(5) 3_665 2_545
O1 K1 Si1 142.31(4) 12_556 2_545
O1 K1 Si1 92.10(4) 14_556 2_545
O1 K1 Si1 85.73(4) 24_654 2_545
O1 K1 Si1 131.93(4) 2_654 2_545
Si1 K1 Si1 113.70(2) . 2_545
Si1 K1 Si1 103.68(3) 13_655 2_545
O1 K1 Si1 145.47(5) 15_546 3_665
O1 K1 Si1 27.53(4) 10_666 3_665
O2 K1 Si1 90.47(5) 2_545 3_665
O2 K1 Si1 28.15(5) 3_665 3_665
O1 K1 Si1 92.10(4) 12_556 3_665
O1 K1 Si1 142.31(4) 14_556 3_665
O1 K1 Si1 131.93(4) 24_654 3_665
O1 K1 Si1 85.73(4) 2_654 3_665
Si1 K1 Si1 113.70(2) . 3_665
Si1 K1 Si1 103.68(3) 13_655 3_665
Si1 K1 Si1 117.95(4) 2_545 3_665
O1 K2 O1 143.02(3) 15_556 5_564
O1 K2 O1 101.27(7) 15_556 6_554
O1 K2 O1 66.64(5) 5_564 6_554
O1 K2 O1 66.64(5) 15_556 14_566
O1 K2 O1 101.27(7) 5_564 14_566
O1 K2 O1 143.02(3) 6_554 14_566
O1 K2 O1 66.64(5) 15_556 13_666
O1 K2 O1 143.02(3) 5_564 13_666
O1 K2 O1 143.02(3) 6_554 13_666
O1 K2 O1 66.64(5) 14_566 13_666
O1 K2 O1 143.02(3) 15_556 4_664
O1 K2 O1 66.64(5) 5_564 4_664
O1 K2 O1 66.64(5) 6_554 4_664
O1 K2 O1 143.02(3) 14_566 4_664
O1 K2 O1 101.27(7) 13_666 4_664
O1 K2 O3 52.10(4) 15_556 2
O1 K2 O3 116.35(5) 5_564 2
O1 K2 O3 52.10(4) 6_554 2
O1 K2 O3 116.35(5) 14_566 2
O1 K2 O3 99.81(5) 13_666 2
O1 K2 O3 99.81(5) 4_664 2
O1 K2 O3 99.81(5) 15_556 1_565
O1 K2 O3 52.10(4) 5_564 1_565
O1 K2 O3 99.81(5) 6_554 1_565
O1 K2 O3 52.10(4) 14_566 1_565
O1 K2 O3 116.35(5) 13_666 1_565
O1 K2 O3 116.35(5) 4_664 1_565
O3 K2 O3 120.0 2 1_565
O1 K2 O3 116.35(5) 15_556 3_665
O1 K2 O3 99.81(5) 5_564 3_665
O1 K2 O3 116.35(5) 6_554 3_665
O1 K2 O3 99.81(5) 14_566 3_665
O1 K2 O3 52.10(4) 13_666 3_665
O1 K2 O3 52.10(4) 4_664 3_665
O3 K2 O3 120.000(1) 2 3_665
O3 K2 O3 120.000(1) 1_565 3_665
O1 K2 Sm2 140.64(3) 15_556 16_556
O1 K2 Sm2 39.37(3) 5_564 16_556
O1 K2 Sm2 39.37(3) 6_554 16_556
O1 K2 Sm2 140.63(3) 14_566 16_556
O1 K2 Sm2 140.63(3) 13_666 16_556
O1 K2 Sm2 39.36(3) 4_664 16_556
O3 K2 Sm2 90.0 2 16_556
O3 K2 Sm2 90.0 1_565 16_556
O3 K2 Sm2 90.0 3_665 16_556
O1 K2 Sm2 39.37(3) 15_556 .
O1 K2 Sm2 140.63(3) 5_564 .
O1 K2 Sm2 140.63(3) 6_554 .
O1 K2 Sm2 39.37(3) 14_566 .
O1 K2 Sm2 39.37(3) 13_666 .
O1 K2 Sm2 140.63(3) 4_664 .
O3 K2 Sm2 90.0 2 .
O3 K2 Sm2 90.0 1_565 .
O3 K2 Sm2 90.0 3_665 .
Sm2 K2 Sm2 180.0 16_556 .
O1 K2 Si1 25.71(4) 15_556 2
O1 K2 Si1 130.68(4) 5_564 2
O1 K2 Si1 75.87(4) 6_554 2
O1 K2 Si1 89.71(4) 14_566 2
O1 K2 Si1 85.46(4) 13_666 2
O1 K2 Si1 125.28(4) 4_664 2
O3 K2 Si1 26.98(2) 2 2
O3 K2 Si1 107.91(6) 1_565 2
O3 K2 Si1 125.71(6) 3_665 2
Sm2 K2 Si1 115.137(13) 16_556 2
Sm2 K2 Si1 64.863(13) . 2
O2 K3 O2 180.00(11) 15_445 3_665
O2 K3 O2 68.00(8) 15_445 14_565
O2 K3 O2 112.00(8) 3_665 14_565
O2 K3 O2 112.00(8) 15_445 2_545
O2 K3 O2 68.00(8) 3_665 2_545
O2 K3 O2 180.00(10) 14_565 2_545
O2 K3 O2 68.00(8) 15_445 13_655
O2 K3 O2 112.00(8) 3_665 13_655
O2 K3 O2 68.00(8) 14_565 13_655
O2 K3 O2 112.00(8) 2_545 13_655
O2 K3 O2 112.00(8) 15_445 1_455
O2 K3 O2 68.00(8) 3_665 1_455
O2 K3 O2 112.00(8) 14_565 1_455
O2 K3 O2 68.00(8) 2_545 1_455
O2 K3 O2 180.00(10) 13_655 1_455
O2 K3 K1 54.391(12) 15_445 13
O2 K3 K1 125.609(12) 3_665 13
O2 K3 K1 54.391(12) 14_565 13
O2 K3 K1 125.609(12) 2_545 13
O2 K3 K1 108.52(5) 13_655 13
O2 K3 K1 71.48(5) 1_455 13
O2 K3 K1 125.609(12) 15_445 2
O2 K3 K1 54.391(12) 3_665 2
O2 K3 K1 71.48(5) 14_565 2
O2 K3 K1 108.52(5) 2_545 2
O2 K3 K1 125.609(12) 13_655 2
O2 K3 K1 54.391(12) 1_455 2
K1 K3 K1 72.841(15) 13 2
O2 K3 K1 54.391(12) 15_445 14
O2 K3 K1 125.609(12) 3_665 14
O2 K3 K1 108.52(5) 14_565 14
O2 K3 K1 71.48(5) 2_545 14
O2 K3 K1 54.391(12) 13_655 14
O2 K3 K1 125.609(12) 1_455 14
K1 K3 K1 107.159(15) 13 14
K1 K3 K1 180.0 2 14
O2 K3 K1 71.48(5) 15_445 3
O2 K3 K1 108.52(5) 3_665 3
O2 K3 K1 125.609(12) 14_565 3
O2 K3 K1 54.391(12) 2_545 3
O2 K3 K1 125.609(12) 13_655 3
O2 K3 K1 54.391(12) 1_455 3
K1 K3 K1 72.841(15) 13 3
K1 K3 K1 107.159(15) 2 3
K1 K3 K1 72.841(15) 14 3
O2 K3 K1 108.52(5) 15_445 15
O2 K3 K1 71.48(5) 3_665 15
O2 K3 K1 54.391(12) 14_565 15
O2 K3 K1 125.609(12) 2_545 15
O2 K3 K1 54.391(12) 13_655 15
O2 K3 K1 125.609(12) 1_455 15
K1 K3 K1 107.159(15) 13 15
K1 K3 K1 72.841(15) 2 15
K1 K3 K1 107.159(15) 14 15
K1 K3 K1 180.0 3 15
O2 K3 K1 125.608(12) 15_445 .
O2 K3 K1 54.392(12) 3_665 .
O2 K3 K1 125.608(12) 14_565 .
O2 K3 K1 54.392(12) 2_545 .
O2 K3 K1 71.48(5) 13_655 .
O2 K3 K1 108.52(5) 1_455 .
K1 K3 K1 180.0 13 .
K1 K3 K1 107.160(15) 2 .
K1 K3 K1 72.840(15) 14 .
K1 K3 K1 107.160(15) 3 .
K1 K3 K1 72.840(15) 15 .
O1 Si1 O1 110.48(14) 14_556 12_556
O1 Si1 O2 111.17(8) 14_556 .
O1 Si1 O2 111.17(8) 12_556 .
O1 Si1 O3 106.58(10) 14_556 .
O1 Si1 O3 106.58(10) 12_556 .
O2 Si1 O3 110.67(15) . .
O1 Si1 K1 63.48(7) 14_556 .
O1 Si1 K1 63.48(7) 12_556 .
O2 Si1 K1 167.77(10) . .
O3 Si1 K1 81.56(12) . .
O1 Si1 K1 64.14(7) 14_556 13_655
O1 Si1 K1 64.15(7) 12_556 13_655
O2 Si1 K1 89.20(9) . 13_655
O3 Si1 K1 160.13(12) . 13_655
K1 Si1 K1 78.57(3) . 13_655
O1 Si1 K1 139.79(8) 14_556 2_655
O1 Si1 K1 53.00(7) 12_556 2_655
O2 Si1 K1 59.60(3) . 2_655
O3 Si1 K1 113.24(5) . 2_655
K1 Si1 K1 116.46(2) . 2_655
K1 Si1 K1 76.24(3) 13_655 2_655
O1 Si1 K1 53.00(7) 14_556 3_655
O1 Si1 K1 139.79(8) 12_556 3_655
O2 Si1 K1 59.60(3) . 3_655
O3 Si1 K1 113.24(5) . 3_655
K1 Si1 K1 116.46(2) . 3_655
K1 Si1 K1 76.24(3) 13_655 3_655
K1 Si1 K1 112.42(4) 2_655 3_655
O1 Si1 K2 51.96(7) 14_556 1_545
O1 Si1 K2 133.41(7) 12_556 1_545
O2 Si1 K2 115.42(5) . 1_545
O3 Si1 K2 56.25(4) . 1_545
K1 Si1 K2 70.852(16) . 1_545
K1 Si1 K2 115.965(17) 13_655 1_545
K1 Si1 K2 167.46(3) 2_655 1_545
K1 Si1 K2 69.981(15) 3_655 1_545
O1 Si1 K2 133.41(7) 14_556 7
O1 Si1 K2 51.96(7) 12_556 7
O2 Si1 K2 115.42(5) . 7
O3 Si1 K2 56.25(4) . 7
K1 Si1 K2 70.851(16) . 7
K1 Si1 K2 115.965(17) 13_655 7
K1 Si1 K2 69.982(15) 2_655 7
K1 Si1 K2 167.46(3) 3_655 7
K2 Si1 K2 104.98(2) 1_545 7
Si1 O1 Sm2 167.27(12) 15_556 13_666
Si1 O1 K1 99.47(8) 15_556 14_666
Sm2 O1 K1 89.17(6) 13_666 14_666
Si1 O1 K2 102.32(9) 15_556 13_666
Sm2 O1 K2 86.82(6) 13_666 13_666
K1 O1 K2 90.49(6) 14_666 13_666
Si1 O1 K1 87.86(8) 15_556 15_556
Sm2 O1 K1 83.88(6) 13_666 15_556
K1 O1 K1 172.48(7) 14_666 15_556
K2 O1 K1 86.25(5) 13_666 15_556
Si1 O1 K1 87.53(8) 15_556 3_666
Sm2 O1 K1 82.77(5) 13_666 3_666
K1 O1 K1 92.34(6) 14_666 3_666
K2 O1 K1 169.17(7) 13_666 3_666
K1 O1 K1 89.66(6) 15_556 3_666
Si1 O2 Sm1 140.53(14) . 1_655
Si1 O2 K3 129.28(12) . 1_655
Sm1 O2 K3 90.19(7) 1_655 1_655
Si1 O2 K1 92.25(5) . 3_655
Sm1 O2 K1 98.03(5) 1_655 3_655
K3 O2 K1 76.59(5) 1_655 3_655
Si1 O2 K1 92.25(5) . 2_655
Sm1 O2 K1 98.03(5) 1_655 2_655
K3 O2 K1 76.59(5) 1_655 2_655
K1 O2 K1 148.64(9) 3_655 2_655
Si1 O3 Si1 136.8(2) 16_556 .
Si1 O3 K2 96.770(14) 16_556 1_545
Si1 O3 K2 96.770(14) . 1_545
Si1 O3 K2 96.770(14) 16_556 7
Si1 O3 K2 96.770(14) . 7
K2 O3 K2 142.66(12) 1_545 7
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sm1 O2 2.338(2) 18_666
Sm1 O2 2.338(2) 2_545
Sm1 O2 2.338(2) 1_455
Sm1 O2 2.338(2) 3_665
Sm1 O2 2.338(2) 17_546
Sm1 O2 2.338(2) 16_456
Sm1 K3 3.62110(8) .
Sm1 K3 3.62110(8) 4
Sm1 K1 4.0279(8) 3
Sm1 K1 4.0279(8) 16_556
Sm1 K1 4.0279(8) 17_556
Sm1 K1 4.0279(8) 18_556
Sm2 O1 2.3003(17) 24_664
Sm2 O1 2.3003(17) 15_556
Sm2 O1 2.3003(17) 23_564
Sm2 O1 2.3003(17) 14_566
Sm2 O1 2.3003(17) 22_554
Sm2 O1 2.3003(17) 13_666
Sm2 K1 3.5867(5) 14_565
Sm2 K1 3.5867(5) 1_565
Sm2 K1 3.5867(5) 13_665
Sm2 K1 3.5867(5) 2
Sm2 K1 3.5867(5) 3_665
Sm2 K1 3.5867(5) 15
K1 O1 2.7853(19) 15_546
K1 O1 2.7853(19) 10_666
K1 O2 2.9696(9) 2_545
K1 O2 2.9696(9) 3_665
K1 O1 3.008(2) 12_556
K1 O1 3.008(2) 14_556
K1 O1 3.057(2) 24_654
K1 O1 3.057(2) 2_654
K1 Si1 3.3593(11) .
K1 Si1 3.3938(11) 13_655
K1 Si1 3.4402(6) 2_545
K1 Si1 3.4402(6) 3_665
K2 O1 2.9271(19) 15_556
K2 O1 2.9271(19) 5_564
K2 O1 2.9271(19) 6_554
K2 O1 2.9271(19) 14_566
K2 O1 2.9271(19) 13_666
K2 O1 2.9271(19) 4_664
K2 O3 3.0399(11) 2
K2 O3 3.0399(11) 1_565
K2 O3 3.0399(11) 3_665
K2 Sm2 3.62110(8) 16_556
K2 Si1 3.6306(5) 2
K3 O2 2.757(2) 15_445
K3 O2 2.757(2) 3_665
K3 O2 2.757(2) 14_565
K3 O2 2.757(2) 2_545
K3 O2 2.757(2) 13_655
K3 O2 2.757(2) 1_455
K3 K1 3.5529(9) 13
K3 K1 3.5529(9) 2
K3 K1 3.5529(9) 14
K3 K1 3.5529(9) 3
K3 K1 3.5529(9) 15
Si1 O1 1.6122(18) 14_556
Si1 O1 1.6122(18) 12_556
Si1 O2 1.624(2) .
Si1 O3 1.6589(16) .
Si1 K1 3.3938(11) 13_655
Si1 K1 3.4402(6) 2_655
Si1 K1 3.4402(6) 3_655
Si1 K2 3.6307(5) 1_545
Si1 K2 3.6307(5) 7
O1 Si1 1.6122(18) 15_556
O1 Sm2 2.3002(17) 13_666
O1 K1 2.7854(19) 14_666
O1 K2 2.9271(19) 13_666
O1 K1 3.008(2) 15_556
O1 K1 3.057(2) 3_666
O2 Sm1 2.338(2) 1_655
O2 K3 2.757(2) 1_655
O2 K1 2.9695(9) 3_655
O2 K1 2.9695(9) 2_655
O3 Si1 1.6588(16) 16_556
O3 K2 3.0399(11) 1_545
O3 K2 3.0399(11) 7
